Spreadsheet: 2356dacc-60fb-41cd-9075-114092c0521a
Sheet: 6. F22... & CrMo

 |  |  |  |  | MD-SLS; Part of SOP
M-spec |  | Linked standards |  | Material / Grade | Dimension limitation | Product | Certificate |  | Delivered condition |  |  |  |  | Chemical composition |  |  |  |  | Yield & Tensile |  |  |  |  |  |  |  |  |  | Impact energy |  |  |  | Hardness (maxim) |  | Minimum reduction
 |  | NORSOK | Other |  |  |  |  | Production method | Heat treatment | Temp minimum | Soaking time | Cooling medium | Forged to shape | Cast / Ladle analysis |  | Product analysis |  | CEV | Minimum yield strength |  |  | [NAME] strength |  |  | Ratio | Elongation (minimum) |  |  | Temp | Dim | Energy J
 | rev. |  |  |  | m m |  |  |  |  | ºC (F) |  |  |  | Element | Content % | Element | Content % |  | Dimension mm | KSI | MPa | Dimension mm | KSI | MPa | % | Dimension mm | % | Reduction of area | ºC | m m | average | single | Test material | Raw material
M10805 | K |  | ASTM A694 FMC Q01206 | F65 | Prior to heat treatment:  <75mm (<3")  weight lim: 500 pounds | forged or rolled steel pipe flanges, hubs, fittings and parts |  |  | Alt A: Austenitize**  Temper   Alt B (incr. [NAME]) Normalize*  Austenitize**  Temper   Alt C:(incr. [NAME]) Austenitize*/**  Austenitize**  Temper | Alt A: 913 - 968 (1675 - 1775) 538 - 690 (1000 - 1275)  Alt B 925 - 982 (1700 - 1800) 913 - 968 (1675 - 1725) 538 - 690 (1000 - 1275)  Alt C: 954 - 982 (1750 - 1800) 885 - 940 (1625 - 1725) 538 - 690 (1000 - 1275) | * min. 15 minutes/inch  [NAME] times may be shorter than those required by Q01207 but shall be 15 minutes/inch minimum no matter how the temperature is measured. | ** followed by Water Quench |  | C Mn Cr Ni P S N V Nb Mo Cu V+Nb+Ti Si B Fe | 0.15 - 0.20 1.15 - 1.4 max 0.3 max 0.4 max 0.025 max 0.025 0.01 - 0.030 0.07 - 0.11 max 0.02 max 0.12 max 0.40 max 0.12 max 0.35 Not intentionally added Balance | C Mn Cr Ni P S N V Nb Mo Cu V+Nb+Ti Si B Fe | 0.14 - 0.21 1.11 - 1.44 max 0.3 max 0.43 [NAME] 0.030 [NAME] 0.030 max 0.040 0.06 - 0.13 max 0.02 [NAME] 0.13 max 0.43 max 0.12 max 0.35 Not intentionally added Balance | 0.40 - 0.45 |  | 65 | 450 |  | 77 | 530 |  |  | 20 | 35 | -18 (0 F) |  | 40 (30 ft.lbf) | 27 (20 ft.lbf) | 174 - 237 HBW
M10805 | J |  | ASTM A694 FMC Q01206 | F65 | Prior to heat treatment:  <75mm (<3")  weight lim: 500 pounds | forged or rolled steel pipe flanges, hubs, fittings and parts |  |  | Alt A: Austenitize**  Temper   Alt B (incr. [NAME]) Normalize*  Austenitize**  Temper   Alt C:(incr. [NAME]) Austenitize*/**  Austenitize**  Temper | Alt A: 913 - 968 (1675 - 1775) 538 - 690 (1000 - 1275)  Alt B 925 - 982 (1700 - 1800) 913 - 968 (1675 - 1725) 538 - 690 (1000 - 1275)  Alt C: 954 - 982 (1750 - 1800) 885 - 940 (1625 - 1725) 538 - 690 (1000 - 1275) | * min. 15 minutes/inch | ** followed by Water Quench |  | C Mn Cr Ni P S N V Nb Mo Cu V+Nb+Ti Si B Fe | 0.15 - 0.20 1.15 - 1.4 max 0.3 max 0.4 max 0.025 max 0.025 0.01 - 0.030 0.07 - 0.11 max 0.02 max 0.12 max 0.40 max 0.12 max 0.35 Not intentionally added Balance | C Mn Cr Ni P S N V Nb Mo Cu V+Nb+Ti Si B Fe | 0.14 - 0.21 1.11 - 1.44 max 0.3 max 0.43 [NAME] 0.030 [NAME] 0.030 max 0.040 0.06 - 0.13 max 0.02 [NAME] 0.13 max 0.43 max 0.12 max 0.35 Not intentionally added Balance | 0.40 - 0.45 |  | 65 | 450 |  | 77 | 530 |  |  | 20 | 35 | -18 (0 F) |  | 40 (30 ft.lbf) | 27 (32 ft.lbf) | 174 - 237 HBW
M10806 | A |  | ASTM A694 API 5L | F65 X65 |  | forged or rolled hollow sections | EN 10204 Type 3.1 or higher |  | Liquid quench Tempered  alt: stress reieve for 4 hours | min 650    630 |  |  |  | C P S V Nb V+Nb+Ti Fe | [NAME] 0.16 max 0.015 [NAME] 0.010 max 0.06 [NAME] 0.04 max 0.10 Balance | C P S V Nb V+Nb+Ti Fe | [NAME] 0.16 max 0.015 [NAME] 0.010 max 0.06 [NAME] 0.04 max 0.10 Balance | [NAME] 0.43 |  | 65 | 450 |  | 77 | 530 |  |  | 20 |  | -46 |  | 40 | 30 | 237 HB 22 HRC |  | 4:1
M11919 | A |  | API SPEC 7, sect. TOOL JOINTS  EN ISO 13628-7  ISO 10423/ API Spec 6A | CrMo-steel |  | Wrought bar, hollow bar, tubulars, and forgings for workover risers  -Not suited for welding -Not suited for sour service | EN 10204 Type 3.1 or higher | fully killed and produced in accordance with a fine grain melting practice  hot worked | Liquid quenched and tempered | Recorded & reported on Matherial Certificate | Recorded & reported on Matherial Certificate |  |  | CrMo-Steel with: C P S  A complete list of all alloying elements with min/[NAME] limits and the maximum content of relevant residual elements shall be proposed by the anufacturer and submitted to FMC for approval prior to start of production | [NAME] 0.40 [NAME] 0.025 max 0.015 |  |  | Not suited for welding |  | 120 - 131 | 827 - 900 |  | 140 | 965 | 0.92 | L=5D: | 16 | 35 | -20 (-4) | Long. &  Transv. | 42 | 32 | 285 - 333 HBW 30 - 35 HRC | 285 - 333 HBW 30 - 35 HRC | 4:1
M20164 | B |  | API 6A (PSL 3)  ASTM A370  ASTM A991  (ASTM A182) (MDS*94) | F22   AISI 4340  Low alloy steel |  | forgings or hot rolled bar for connector items and other critical, heavily loaded components - Rod shaped parts may be produced by hot rolling and cold drawn instead of forging, and followed by heat treatment. | EN 10204 Type 3.1 or higher |  | liquid quenched and temperes | x |  |  |  | P  S | [NAME] 0.025 [NAME] 0.025 | P  S | [NAME] 0.025 [NAME] 0.025 |  |  | 95 - 123 | 645 - 850 |  | 120 | 828 |  |  | 18 | 35 | -20 (-4) |  | 42 | 32 | 250 - 300 HB | 250 - 300 HB | 4:1
M20164 | A |  | API 6A  (ASTM A182) (MDS*94) | F22   Low alloy steel  alternatively: AISI 4340 |  | forgings and hot rolled bar for connector items and other critical, heavily loaded components | EN 10204 Type 3.1 or higher |  | liquid quenched and temperes | x |  |  |  | P  S | [NAME] 0.025 [NAME] 0.025 | P  S | [NAME] 0.025 [NAME] 0.025 |  |  | 95 - 123 | 645 - 850 |  | 120 | 828 |  |  | 18 | 35 | -20 (-4) |  | 42 | 32 | 250 - 300 HB | 250 - 300 HB | 4:1
M20413 | A |  | ASTM A29 type    API 6A  Former  MDS-0000093 | AISI 8630  PSL 3 |  | Forgings | EN 10204 Type 3.1 or higher | Fine grain melting practice | liquid quenched and tempered | 640°C. |  |  |  | Carbon Phosphorus Sulfur Chromium Molybdenum Hydrogen (ladle) Manganese Nickel Silicon Vanadium Copper Titanium Aluminum | 0,25 - 0,33 [NAME] 0,025 max 0,025 0,85 -1,00 0,35 - 0,45 [NAME] 2,0 ppm 0,70 – 1,10 0,75 – 0,90 0,15 – 0,35 max 0,06 max 0,25 max 0,06 [NAME] 0,035 |  |  |  |  | 75 | 517 |  | 95 | 655 |  |  | 18 | 35 | -20 (-4) |  | 42 | 32 | 207 - 237 HB | 207 - 237 HB | 3:1
M20714 | C |  | ASTM A182 API 6A (PLS 3) | F22  Low alloy [NAME]-steel |  | Forgings | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched  tempered |  |  |  | Flanged part as close to final shape as possible | C P S Cr Mo Mn Si H Fe | 0.05-0.20 [NAME] 0.025 [NAME] 0.025 2.0 – 2.5 0.87 – 1.13 0.30 - 0.60 0.50 max 0.002 (2.0 ppm) Balance | C P (M-spec) S (M-spec) [NAME] Mn Si Fe | 0.04-0.21 max 0.025 [NAME] 0.025 2.0 – 2.5 0.82 – 1.18 0.27 - 0.63 0.55 Balance |  |  | 100 - 123 | 690 - 850 |  | 120 | 828 |  |  | 18 | 35 | -40 |  | 42 | 32 | 235 - 300 HB | 235 - 300 HB | 4:1
M20715 | C |  | ASTM A182  API 6A/ISO 10423 | F22  PSL 3  Low alloy [NAME]-steel |  | Forgings | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched & tempered |  |  |  | Flanged part as close to final shape as possible | Carbon  Mn Phosphorus Sulfur Si Chromium Molybdenum Hydrogen  Fe | 0.05 – 0.20 0.30 - 0.60 max 0.025 [NAME] 0.025 0.50 2.0 – 2.5 0.87 – 1.13 max 2.0 ppm Balance | Carbon  Mn Phosphorus Sulfur Si Chromium Molybdenum Fe | 0.04 – 0.21 0.27 - 0.63 [NAME] 0.030 [NAME] 0.030 0.55 2.0 – 2.5 0.82 – 1.18 Balance |  |  | 87 - 109 | 600 - 750 |  | 100 | 690 |  |  | 18 | 35 | -40 |  | 42 | 32 | 210 - 300 HB | 210 - 300 HB | 4:1
M20716 | A |  | ASTM A182   API 6A   Former [NAME] | F22 (mod)  PLS 3  Low alloy [NAME]-steel |  | Forgings | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched & tempered | 640°C. |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Hydrogen (ladle)  Fe | 0.05 – 0.15 max 0.025 [NAME] 0.025 2.0 – 2.5 0.87 – 1.13 max 2.0 ppm Balance |  |  |  |  | 80 | 551 |  | 100 | 689 |  | [NAME]: L0=5xd: | 18 16 | 35 | -40 |  | 42 | 32 | 207 - 237 HB 18 - 22 HRC | 207 - 237 HB 18 - 22 HRC | 3:1
M20717 | B |  | ASTM A182  API 6A   (MDS-*20222) | F22  Low alloy [NAME]-steel |  | X-tree block hubs valve bodies connector items riser components other critical , heavily loaded or pressure containing comp. | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched  tempered | x |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Mn Si Hydrogen Fe | 0.05 – 0.15 max 0.025 [NAME] 0.025 2.0 – 2.5 0.87 – 1.13 0.30 - 0.60 0.50 max 2.0 ppm Balance | Carbon  Phosphorus Sulfur Chromium Molybdenum Mn Si Fe | 0.040 – 0.16 [NAME] 0.030 [NAME] 0.030 2.0 – 2.5 0.82 – 1.18 0.27 - 0.63 0.55 Balance |  |  | 85 | 586 |  | 100 | 689 |  |  | [NAME]: 18 L0=5xd: 16 | 35 | -40 |  | 42 | 32 | 207 - 237 HB 18 - 22 HRC | 207 - 237 HB 18 - 22 HRC | 3:1
M20718 | C |  | ASTM A182  API 6A | F22  Low alloy [NAME]-steel |  | X-tree block hubs valve bodies connector items riser components other critical , heavily loaded or pressure containing comp. | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched & tempered | x |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Hydrogen | 0.10 – 0.15 max 0.025 [NAME] 0.025 2.0 – 2.5 0.87 – 1.13 max 2.0 ppm | Carbon  Phosphorus Sulfur Chromium Molybdenum | 0.040 – 0.16 [NAME] 0.030 [NAME] 0.030 2.0 – 2.5 0.82 – 1.18 |  |  | 75 - 109 | 517 - 750 |  | 95 | 655 |  | L0=4xd | 18 | 35 | -46 |  | 42 | 32 | 197 - 237 HBW | 207-237 HBW | 4:1
M20718 | B |  | ASTM A182  API 6A | F22  Low alloy [NAME]-steel |  | X-tree block hubs valve bodies connector items riser components other critical , heavily loaded or pressure containing comp. | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched & tempered | x |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Mn Si Hydrogen Fe | 0.05 – 0.15 max 0.025 [NAME] 0.025 2.0 – 2.5 0.87 – 1.13 0.30 - 0.60 0.50 max 2.0 ppm Balance | Carbon  Phosphorus Sulfur Chromium Molybdenum Mn Si Fe | 0.040 – 0.16 [NAME] 0.030 [NAME] 0.030 2.0 – 2.5 0.82 – 1.18 0.27 - 0.63 0.55 Balance |  |  | 75 - 109 | 517 - 750 |  | 95 | 655 |  | L0=4xd | 18 | 35 | -46 |  | 42 | 32 | 197 - 237 HB | 197 - 237 HB | 4:1
M20720 | E |  | API 6A   Former MDS-0000041  ASTM E112  ASTM A182  NACE MR-01-75/ISO 15156 | F22  Lowalloy   2.25-Cr 1-Mo |  | Forgings | SIR205 EN 10204 | The material shall be fully killed and melted in accordance with a fine grain practice, capable of producing ASTM E112 grain size of 5 or finer. | Normalize (if required) :  Air cool:  Austenitize:  Water quench:  Temper:  Air cool or optional quench:  Simulated Post Weld Heat Treatment is required SPWHT: | 927-968°C (1700-1775°F)  Below 204 °C (400°F)  899-941°C (1650 -1725°F)  Below 204 °C (400°F)  Minimum 660ºC (1220°F)      650°C (1200 °F) followd by still air cooling. | 20 hours |  |  | C Mn Cr Mo P S Si Ni V Nb (Cb) Ti Al | [NAME] 0.10 – 0.15 max 0.30 - 0.60 max 2.00 - 2.50 max 0.87 - 1.13 max 0.025 [NAME] 0.025 [NAME] 0.15 - 0.50 [NAME] 0.50 [NAME] 0.03 max 0.01 [NAME] 0.03 [NAME] 0.05 | Total Residual Elements: | max 0.5 |  |  | 75 | 517 |  | 95 | 654 | [NAME] | 2" or 4D | 18 | 35 |  |  |  |  | 197-237HBW (finished part) | 207-237 HBW
M21515 | A |  | API 6A   Former MDS-0000041 | AISI 4130  PSL 3  Low alloy [NAME]-steel |  | Medium loaded or pressure containing components | EN 10204 Type 3.1 or higher | Hot forged | liquid quenched  tempered | 640 |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Manganese Silicon Hydrogen (ladle)  Total residual Fe | 0.28 – 0.33 max 0.025 max 0.025 0.80 - 1.10 0.15 - 0.30 0.40 - 0.60 0.15 - 0.35 max 2.0 ppm 1.00 Balance |  |  |  |  | 60 | 414 |  | 85 | 621 |  |  | 18 | 35 | -20 |  | 42 | 32 | 174 - 237 HB | 174 - 237 HB | 3:1
M21516 | A |  | MDS-0000040 API 6A | Low alloy [NAME]-steel  AISI 4130 |  | Forgings for medium loaded or pressure containing components | EN 10204 Type 3.1 or higher |  | liquid quenched  tempered | 640 |  |  | Flanged part as close to final shape as possible | Carbon  Phosphorus Sulfur Chromium Molybdenum Manganese Silicon Hydrogen (ladle)  Total residual Fe | 0.28 – 0.33 max 0.025 max 0.025 0.80 - 1.10 0.15 - 0.30 0.40 - 0.60 0.15 - 0.35 max 2.0 ppm 1.00 Balance |  |  |  |  | 75 | 517 |  | 100 | 690 |  |  | 18 | 35 | -20 |  | 42 | 32 | 207 - 237 HB 18 - 22 HRC | 207 - 237 HB 18 - 22 HRC | 3:1